Survey

* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project

Survey

Document related concepts

Temperature wikipedia , lookup

Thermal expansion wikipedia , lookup

Time in physics wikipedia , lookup

Electrical resistivity and conductivity wikipedia , lookup

Marie Curie wikipedia , lookup

Condensed matter physics wikipedia , lookup

Perturbation theory wikipedia , lookup

Partial differential equation wikipedia , lookup

Equation of state wikipedia , lookup

Transcript

JOURNAL OF APPLIED PHYSICS 100, 044114 共2006兲 Curie-Weiss law in thin-film ferroelectrics Biao Wang School of Physics and Engineering, Sun Yat-sen University, Guangzhou, China C. H. Wooa兲 Department of Electronic and Information Engineering, The Hong Kong Polytechnic University, Hung Hom, Kowloon, Hong Kong 共Received 20 July 2005; accepted 17 July 2006; published online 31 August 2006兲 The stationary self-polarization field of a thin film in an open circuit is analytically solved for temperatures near the para-/ferroelectric transformation within the Ginzburg-Landau theory. For second-order ferroelectrics, or first-order ferroelectrics with a sufficiently large elastic self-energy of the transformation strain, the solution is real and stable, from which the corresponding electric susceptibility of the film can be derived. A Curie-Weiss-type relation of the permittivity is obtained for both the supercritical and subcritical temperature regimes near the transition. In the paraelectric state, the Curie parameter of the thin film is found to be independent of its thickness, whereas in the ferroelectric state, its magnitude decreases rapidly with decreasing film thickness. © 2006 American Institute of Physics. 关DOI: 10.1063/1.2336979兴 I. INTRODUCTION The large surface to bulk ratio causes ferroelectric thin films to exhibit phase-transition characteristics that are generally different from their bulk counterparts. Indeed, in extreme cases, such as in PbTiO3, BaTiO3, and lead zirconic titanate 共PZT兲 thin films, the ferroelectric transition can even be totally suppressed, when the film thickness is below certain critical values. This dependence of the phase-transition characteristics on the sample size has been investigated using both first-principles calculations1,2 and thermodynamic models.3–5 Experiments have also confirmed that the Curie temperatures of epitaxial films of PbTiO3 grown on SrTiO3 共001兲 substrate decrease rapidly with the film thickness below 50 nm, as predicted theoretically.5,6 Due to the ever-increasing size and complexity of electronic circuitry that has to be packed into the limited space of modern integrated circuit 共ICs兲, the influence of sample size on material properties is a subject of general interest to both scientific and technological investigations.10–12 For the general phase-transition problem of finite size systems, some scaling laws have been established,7–9 and it is not unusual that controlling parameters for phase transitions such as the Curie temperature may differ substantially from those in the bulk materials. In addition, important physical properties may also become sensitive to sample dimensions through the stability of the prevailing phase. In a previous paper,5 we studied the relationship between the film thickness and the Curie temperature of the para-/ ferroelectric transition in a thin film on a rigid substrate. By considering the dynamic stability of the stationary solution of the Ginsberg-Landau equation, simple expressions of the Curie temperature as a function of film thickness were derived without having to go through the complexities of an explicit solution. The order of the transition and the difference between the heat-up and cool-down transition temperaa兲 Electronic mail: [email protected] 0021-8979/2006/100共4兲/044114/5/$23.00 tures, on the other hand, were found to be independent of the film thickness, but might depend on the constraint of the substrate. This conclusion was further investigated in another work,13 in which the Ginzburg-Landau equation for a thin film on a substrate with varying compliance was solved in the neighborhood of the transition temperature. Although the conclusion of Ref. 5 was confirmed, yet for the case of a compliant substrate, Ref. 13 found that the order of transition of a thin film of first-order ferroelectric material did not remain constant, but may indeed change according to the film thickness relative to that of the substrate. In the present paper, we are interested in the effect of the film thickness on the Curie-Weiss law of electric susceptibility. In this calculation, the explicit solution of the GinzburgLandau equation is required, which we obtained via a perturbation series expansion method.13 In Sec. II, the evolution of the ferroelectric thin films is formulated following Wang and Woo5 within the dynamic Ginzburg-Landau theory using the corresponding free energies, in which the local selfpolarization near a free surface is subsumed in the boundary conditions through the “extrapolation length” parameter. The constraint of a rigid substrate is assumed, and we consider electric boundary conditions under which the film is between electrodes from which it is insulated. In Sec. III, the stationary solutions of the Ginzburg-Landau equation are obtained in the neighborhood of the transition temperature, by means of a perturbation series expansion method. The solutions are then used in our investigation in Sec. IV. The paper is summarized and concluded in Sec. V. II. FORMULATION We consider a ferroelectric thin film of dimensions ⬁ ⫻ ⬁ ⫻ h 共i.e., h = film thickness兲 on a rigid substrate, i.e., one with a thickness much larger than h. The origin of the coordinate system is at the center of the cell. We base our formulation on the classical description of electrical susceptibility of a collection of polar molecules, the local polarization Ptotal 100, 044114-1 © 2006 American Institute of Physics Downloaded 20 Mar 2011 to 158.132.161.9. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 044114-2 J. Appl. Phys. 100, 044114 共2006兲 B. Wang and C. H. Woo at any point consists of a permanent molecular component P and an induced component PE. P arises from the permanent electric moment due to the polar nature of the molecular structure/configuration of the material, e.g., its crystallography, in its prevailing para-/ferroelectric phase. P is thus a function of the temperature, the electric field and the mechanical stresses in the sample through its Curie temperature. We call P the self-polarization, instead of “spontaneous polarization” like what we used to Ref. 5, to distinguish it from the more commonly used meaning of the total 共i.e., observed兲 polarization in the absence of an external field. We note that Ptotal and P are equal only when the depolarization field vanishes, such as in the bulk material between shortcircuited electrodes. The induced component PE is the polarizations 共ionic + electronic兲 induced by the total electric field E in the material according to PE = dE, where d is the temperatureindependent component of the susceptibility corresponding to the field-induced part of the polarization. We may identify E, which has its origin from the combined effects of P and Ex, as the sum of the external field Ex and the depolarization field Ed. In this regard, the displacement field in the ferroelectric can be written either in terms of Ptotal or P: D = 0E + Ptotal = 0E + P + dE = dE + P, where 0 is the background permittivity, and d is that part of the permittivity of the ferroelectric corresponding to d. For simplicity the nonzero component of the selfpolarization P of the ferroelectric thin film is assumed to be T orthogonal to the surface of the film. The eigenstrain xx T 2 = yy = QP due to the para-/ferroelectric transition is constrained by the rigid substrate, causing an elastic self-energy 2 / C11兲, C11 Fe = GQ2 兰 兰兰V P4d, where G = 共C11 + C12 − 2C12 and C12 being components of the elastic modulus, and V the volume, of the film. We neglect the effects of the epitaxial stresses to simplify the discussion in the present work. It is clear from Ref. 5 that its inclusion only has the equivalent effect of shifting the bulk transition temperature. Following Ref. 5, with the help of the Ginzburg-Landau functional, the dynamic equation of the self-polarization in the thin film can be written as P ␦F =− = − A共T − TC0兲P − 共B + 4GQ2兲P3 − CP5 M t ␦P d2 P + Ed + D 2 , dz 共1兲 with the boundary conditions, P dP = ⫿ , dz ␦ h z= ± , 2 共2兲 where M is the kinetic coefficient related to the domain wall mobility; A, B, C, and D, are expansion coefficients of the Ginzburg-Landau functional of the homogeneous selfpolarization in the bulk ferroelectric; TC0 is the corresponding Curie temperature; Ed is the depolarizing field, and ␦ is the extrapolation length that describes the near-surface relaxation effect of the local self-polarization.14,15 The meaning of the other symbols are as given in Ref. 5. The electric and polarization fields in the ferroelectric are related through conditions on the boundaries via the laws of electrostatics. In this paper, a ferroelectric thin film in an open circuit is considered, i.e., the film is insulated from the electrodes. In this case, the depolarization field Ed has been derived5 Ed = − P . d 共3兲 Note that the Ed here is different from and generally much larger than that in Ref. 15. Most of bulk ferroelectrics exhibit a first-order phase transition. In such cases, the parameter B is negative, and the parameter C is positive. For bulk materials in which the ferroelectric transition is second order, the parameter B is positive and the higher order terms can be neglected. III. STEADY-STATE SOLUTION NEAR THE BIFURCATION POINT The condition of dynamic stability of the paraelectric state of the evolution equation Eq. 共1兲 has been established,5 from which the critical temperature Tc at which the state becomes unstable can be obtained as a function of the film thickness h: Tc = TC0 − 1 D − kz2 min , Ad A 共4兲 where kz min is the minimum solution of the following transcendental equation: 冉 冊 cot k zh = k s␦ . 2 共5兲 As explained in Ref. 5, Tc is the para-/ferroelectric transition temperature for the thin film. Putting P / t = 0 in Eq. 共1兲, the corresponding stationary equation of the order parameter P can be written as Lc P ⬅ − A共Tc − TC0兲P − 1 d2 P P+D 2 , dz d 共6兲 where Lc is the parabolic operator evaluated at the bifurcation point T = Tc, in the neighborhood of which the solution P is small, if assumed continuous. Following Nicholis and Prigogine,16 both P and ␥ ⬅ T − Tc can be expanded in a power series in terms of a small perturbation from the critical point: P = P1 + 2 P2 + ¯ , ␥ = T − T c = ␥ 1 + 2␥ 2 + ¯ . 共7兲 This expansion is more flexible than the seemingly more natural one in which P is expanded in a power series of 共T − Tc兲.16 More importantly, it allows fractional power dependence of P on 共T − Tc兲. By substituting the expansion 共7兲 into Eq. 共6兲, and equating coefficients of equal powers of , a set of relations of the following form can be obtained: Downloaded 20 Mar 2011 to 158.132.161.9. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 044114-3 J. Appl. Phys. 100, 044114 共2006兲 B. Wang and C. H. Woo 共8兲 k = 1,2, ¯ , L c P k = a k, which have to be satisfied together with the boundary and the initial conditions: Pk dPk = ⫿ , dz ␦ h z= ± . 2 共9兲 The first several coefficients ak are FIG. 1. Schematic of bifurcation diagram for ferroelectric thin film. a1 = 0, a2 = A␥1 P1 , 共10兲 It is easy to check that under the boundary condition 共9兲, the operator Lc is self-adjoint, and 共Lc P*, Pk兲 = 冕 h/2 PkLc P*dz −h/2 = 共P*,Lc Pk兲 冕 h/2 共11兲 P*akdz = 0, −h/2 where P* is the solution of the following homogeneous equation: Lc P* = 0, P* dP* = ⫿ , dz ␦ h z= ± , 2 共12兲 Eq. 共11兲 can be used to determine the coefficients ␥i. Then from the second relation of Eq. 共7兲, one can determine as a function of 共T − Tc兲. Substituting the resulting into the first relation of Eq. 共7兲 and solving the inhomogeneous equations 共9兲 results in an explicit expression for the solution P. Let us consider the ␦ ⬎ 0 case, which is satisfied by most ferroelectrics. Equation 共4兲 dictates that the transition temperature of the thin film is lower than that of the bulk material. The solution of Eq. 共12兲 can be written as P* = M cos共z兲 + N sin共z兲, 共13兲 where  = 冑A共TC0 − Tc兲/D − 1/dD. 共14兲 Suppose the P is distributed symmetrically along the thickness direction, i.e., dP* / dz = 0 at z = 0, then N = 0, and the solution 共13兲 becomes P* = M cos共z兲. 共15兲 Similarly, the solution of the first equation in Eq. 共8兲 can be obtained in the same form as P*. Thus, P1 = M cos共z兲. 共16兲 By using the orthogonal condition in Eq. 共11兲, ␥1 and ␥2 can be determined, ␥1 = 0 since 冕 h/2 −h/2 P1 P*dz = 冕 h/2 −h/2 P21dz ⫽ 0. 共17兲 冕 冕 P41dz −h/2 h/2 . 共18兲 P21dz −h/2 If the corresponding bulk ferroelectrics transition is of second order, i.e., B ⬎ 0, B + 4GQ2 is also positive, and substitution of Eq. 共18兲 into 共7兲 gives = ± = 共P*,ak兲 = B + 4GQ A ␥2 = − a3 = A␥1 P2 + A␥2 P1 + 共B + 4GQ2兲P31 . 2 h/2 冉 冊 Tc − T − ␥2 1/2 for T ⬍ Tc , 共19兲 i.e., the solution is defined in the supercritical 共ferroelectric兲 regime. According to Theorem 3.1 for the bifurcation of a simple eigenvalue,17 the bifurcating solutions are both asymptotically stable in the supercritical regime. The phase diagram for this case is shown in Fig. 1共a兲. Thus, if the bulk ferroelectrics exhibits second-order phase transition, their thin-film counterparts will also exhibit the same order of phase transition, and the universal critical exponents remain unchanged. On the other hand, if the corresponding transition in the bulk material is first order, i.e., B ⬍ 0, then depending on the magnitude of the elastic self-energy of the transformation volume 4GQ2, which is positive definite and has a magnitude of the same order as B, B + 4GQ2 can be either positive or negative. When 4GQ2 is sufficiently large, B + 4GQ2 is positive definite, as in BaTiO3 and PbTiO3, then a first-order bulk ferroelectrics becomes second-order one in a rigidly constrained thin film. This is consistent with the results of Pertsev et al.18 For the two classical perovskite ferroelectrics, BaTiO3 and PbTiO3, these authors also found that the twodimensional clamping of the film could result in a change of transition order. Nevertheless, the results of Ref. 18 should be interpreted noting the assumption that the gradient terms in the free energy were negligible. If the transformation volume satisfies B + 4GQ2 = 0, the solution will include higher order terms of expansions, and thus the critical exponents will differ from their bulk counterpart. If B + 4GQ2 is negative, substitution of Eq. 共18兲 into Eq. 共7兲 gives ⯝ ± 冉 冊 T − Tc ␥2 1/2 for T ⬎ Tc , 共20兲 i.e., the solution is defined only in the subcritical 共paraelectric兲 regime, and both branches are unstable. Physically, there is a maximum value of Tmax above which only one solution is admissible. Therefore, the subcritical branches have to turn, at some value Tmax, in the direction of decreas- Downloaded 20 Mar 2011 to 158.132.161.9. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 044114-4 J. Appl. Phys. 100, 044114 共2006兲 B. Wang and C. H. Woo ing temperature 关Fig. 1共b兲兴. Thus, the solution of P near the critical point can be obtained in the form as P = P 1 = 冦 ±M cos共z兲 ±M cos共z兲 冉 冊 冉 冊 Tc − T − ␥2 1/2 T − Tc ␥2 1/2 , B + 4GQ2 ⬎ 0 and T ⬍ Tc , B + 4GQ2 ⬍ 0 and T ⬎ Tc . 冧 共21兲 It is clear from Eq. 共21兲 that for rigidly constrained thin-film ferroelectrics the order of transitions is independent of its thickness, but depends on the elastic self-energy of the transformation strain under the constraint of the substrate. Furthermore, we note that the second solution in Eq. 共21兲 is unstable, and the actual transition is discontinuous. The behavior of the self-polarization P in the foregoing discussions agrees completely with that derived earlier using linear stability analysis.5 Of course, the solution of P in Eq. 共21兲 cannot be obtained in Ref. 5. 冦 关A + 3共B + 4GQ2兲M 2 cos2共z兲/␥2兴共T − Tc兲 s−1 = for T ⬍ Tc , A共T − Tc兲 for T ⬎ Tc . 冧 共26兲 The average value of s cannot be integrated analytically, such as the average value of the reciprocal. Thus, 具s−1典 = 1 h 冕 h/2 s−1dz −h/2 冦 3共Tc − T兲 =A 1− h 冋 冕 冕 h/2 关 cos2共z兲dz兴2 −h/2 h/2 −h/2 cos 共z兲dz 4 冧 共T − Tc兲 = A 1 − 3共Tc − T兲 ⫻ 册 4 sin2共h兲 + 8h sin共h兲 + 42h2 共T − Tc兲, h sin共2h兲 + 8h sin共h兲 + 62h2 共27兲 IV. DIELECTRIC SUSCEPTIBILITY OF FERROELECTRIC FILMS NEAR THE CRITICAL POINT The susceptibility total of a ferroelectric material measures the response of the total 共i.e., observable兲 polarization in an external field, and is defined by total = 冏 冏 Ptotal Eext 共22兲 . Eext→0 For the present boundary conditions, it can be shown from the laws of electrostatics, total = 1 d 冉冏 冏 P Eext Eext→0 冊 + d ⬅ 1 共 + d兲, d s 共23兲 where d is the dielectric constant 共=d / 0兲. It is sufficient to calculate s, which is much larger than d near the transition temperature. s can be calculated via the total free energy as usual, s−1 = 2 f P2 = A共T − TC0兲 + 1 + 3共B + 4GQ2兲P2 + 5CP4 + D2 d = A共T − Tc兲 + 3共B + 4GQ2兲P2 + 5CP4 . where 共x兲 = 0 for x ⬍ 0, and 共x兲 = 1 for x ⬎ 0 is the step function. Equation 共27兲 may be rewritten in the form 具s−1典−1 = A−1⌰−1共h兲 . 共T − Tc兲 共28兲 Equation 共28兲 shows that, on both sides of the transition temperature, the Curie-Weiss law holds, and that the average susceptibility of the film diverges with a critical exponent of −1. In addition, the corresponding Curie parameter −1 −1 −1 d A ⌰ 共h兲 also changes sign discontinuously across the transition temperature. Both aspects of its behavior are the same as the bulk counterpart. However, for films of finite thickness, the magnitude of the Curie parameter varies according to the thickness, leading to asymmetric divergences across the transition temperature. Indeed, the Curie parameter is independent of the film thickness 共⌰−1 = 1兲 on the paraelectric side 共T ⬎ Tc兲, a well known fact, but depends on the film thickness on the ferroelectric side. Taking the limits in Eq. 共27兲 and using the relations between  and h derived in Ref. 5, it can be shown that the value of ⌰−1 depends on the film thickness h, approaching −关1 − 共8␦ / 3h兲兴 for thick films 共h Ⰷ ␦兲, and −0.5关1 + 共h2 / 5␦2兲兴 for thin films 共h Ⰶ ␦兲. 共24兲 In deriving Eq. 共24兲, we have used Eqs. 共4兲 and 共13b兲 and the following relations: 冉 冊 冋 冉 冊册 冉 冊 2 P P2 z 2 = z P P P z z =2 2 2 P z 3 P = 2 P z2 P z3 共25兲 For positive B + 4GQ2, substitution of the first equation of 共21兲, and  in Eq. 共13b兲, into Eq. 共24兲 yields the inverse susceptibility near Tc, FIG. 2. Normalized susceptibility vs the temperature. Downloaded 20 Mar 2011 to 158.132.161.9. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions 044114-5 J. Appl. Phys. 100, 044114 共2006兲 B. Wang and C. H. Woo TABLE I. Phenomenological parameters of PbTiO3 共in cgs unit兲. ␦ Material To0 共K兲 A 10−5 D 10−15 nm ␣ PbTiO3 763 8.37 3 5 210 transition temperature was derived using a perturbation approach. It was found that the order of the transition and the critical exponents can be changed by the constraint of the substrate. A Curie-Weiss-type relation of dielectric permittivity was obtained in both the supercritical and subcritical regions. It was found that in paraelectric state, the Curie parameter is independent of the film thickness, and remains the same as their bulk counterpart. In the ferroelectric state, on the other hand, the magnitude of the Curie parameter of the film decreases rapidly as its thickness decreases. FIG. 3. The normalized Curie-Weiss parameter −关⌰共h兲兴−1 vs the film thickness h for PbTiO3. Accordingly, for a film thickness of h = 8␦, the Curie param−1 eter −1 of the ferroelectric phase would have dropped d ⌰ 33%. These characteristics are shown in Fig. 2, where the normalized susceptibility, i.e., ⌰−1 / 共T − Tc兲 as a function of temperature, is compared between thick films 共h → ⬁兲 and thin films 共h → 0兲. We note that 具total典 also has a similar relation to T − Tc, as discussed in the foregoing. From the free energy expression in Ref. 5, the contribution from the upper and lower surfaces of the ferroelectric thin film increases the susceptibility according to ⌬ = 2␦ , D 共29兲 which is negligible near the transition temperature. In the following, we consider the example of a well known ferroelectric PbTiO3, the material constants of which are shown in Table I.5 The normalized Curie parameter −关⌰共h兲兴−1 is plotted against the film thickness h in Fig. 3, in which the Curie temperature was obtained as a function of h by using Eqs. 共4兲 and 共5兲. It can be seen that the magnitude of the normalized Curie parameter does decrease rapidly from 1 to 0.5 with decreasing thickness. Indeed, for films of PbTiO3 about 40 nm 共=8␦兲, the ferroelectric transition is accompanied with a decrease of the Curie parameter of about 33%. Similar behavior is also found experimentally for BST films.19 A review on the properties of ferroelectric materials was given in references.20–22 V. SUMMARY AND CONCLUSIONS In this paper, the explicit solution of the steady-state Ginzburg-Landau equation for a ferroelectric film near the ACKNOWLEDGMENTS This project was supported by grants from the Research Grants Council of the Hong Kong Special Administrative Region 共PolyU5322/04E and 5312/03E兲 Natural Science Foundation 共10572兲. J. Junquera and Ph. Ghosez, Nature 共London兲 422, 506 共2003兲. Ph. Ghosez and K. M. Rabe, Appl. Phys. Lett. 76, 2767 共2000兲. Y. G. Wang, W. L. Zhong, and P. L. Zhang, Phys. Rev. B 51, 17235 共1995兲. 4 D. R. Tilley, in Ferroelectric Thin Films: Synthesis and Basic Properties, edited by C. Paz de Araujo, J. F. Scott, and G. W. Taylor 共Taylor and Francis, Oxford, 1996兲, p. 11. 5 B. Wang and C. H. Woo, J. Appl. Phys. 97, 084109 共2005兲. 6 S. K. Streiffer et al., Phys. Rev. Lett. 89, 067601 共2002兲. 7 M. E. Fisher and M. Barber, Phys. Rev. Lett. 28, 1516 共1972兲. 8 D. P. Landau, Phys. Rev. B 14, 255 共1976兲. 9 D. P. Landau and K. Binder, J. Appl. Phys. 63, 3077 共1988兲. 10 S. Li, J. A. Eastman, J. M. Vetrone, C. H. Foster, R. E. Newnham, and L. E. Cross, Jpn. J. Appl. Phys., Part 1 36, 5169 共1997兲. 11 W. L. Zhong, Y. G. Wang, P. L. Zhang, and B. D. Qu, Phys. Rev. B 50, 698 共1994兲. 12 I. P. Batra, P. Wurfel, and B. D. Silverman, Phys. Rev. Lett. 30, 384 共1973兲. 13 B. Wang and C. H. Woo, Acta Mater. 52, 5639 共2004兲. 14 P. G. de Gennes, Superconductivity of Metals and Alloys 共Benjamin, New York, 1966兲, p. 227. 15 R. Kretschmer and K. Binder, Phys. Rev. B 20, 1065 共1979兲. 16 G. Nicolis and I. Prigogine, Self-organization in Nonequilibrium Systems 共Wiley, New York, 1977兲, p. 85. 17 D. H. Sattinger, Group Theoretic Methods in Bifurcation Theory 共Springer-Verlag, Berlin, 1979兲. 18 N. A. Pertsev, A. G. Zembilgotov, and A. K. Tagantsev, Phys. Rev. Lett. 80, 1988 共1998兲. 19 S. K. Streiffer, C. Basceri, C. B. Parker, S. E. Lash, and A. I. Kingon, J. Appl. Phys. 20, 4565 共1999兲. 20 A. K. Tagantsev, V. O. Sherman, K. F. Astafiev, J. Venkatesh, and N. Setter, J. Electroceram. 11, 5 共2003兲. 21 A. K. Tagantsev, V. O. Sherman, K. F. Astafiev, J. Venkatesh, and N. Setter, J. Electroceram. 14, 199 共2005兲. 22 B. Wang and C. H. Woo, J. Appl. Phys. 94, 4053 共2003兲. 1 2 3 Downloaded 20 Mar 2011 to 158.132.161.9. Redistribution subject to AIP license or copyright; see http://jap.aip.org/about/rights_and_permissions